Hindawi Publishing Corporation e Scientiﬁc World Journal Volume 2014, Article ID 526346, 10 pages http://dx.doi.org/10.1155/2014/526346
Research Article Mechanical and Physical Properties of Polyester Polymer Concrete Using Recycled Aggregates from Concrete Sleepers Francisco Carrión, Laura Montalbán, Julia I. Real, and Teresa Real Department of Transportation Engineering and Infrastructures, School of Civil Engineering, Polytechnic University of Valencia, 14 Camino de Vera, 46022 Valencia, Spain Correspondence should be addressed to Francisco Carri´on; [email protected]
Received 12 May 2014; Revised 1 August 2014; Accepted 6 August 2014; Published 27 August 2014 Academic Editor: Sakdirat Kaewunruen Copyright © 2014 Francisco Carri´on et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited. Currently, reuse of solid waste from disused infrastructures is an important environmental issue to study. In this research, polymer concrete was developed by mixing orthophthalic unsaturated polyester resin, artificial microfillers (calcium carbonate), and waste aggregates (basalt and limestone) coming from the recycling process of concrete sleepers. The variation of the mechanical and physical properties of the polymer concrete (compressive strength, flexural strength, modulus of elasticity, density, and water absorption) was analyzed based on the modification of different variables: nature of the recycled aggregates, resin contents (11 wt%, 12 wt%, and 13 wt%), and particle-size distributions of microfillers used. The results show the influence of these variables on mechanical performance of polymer concrete. Compressive and flexural strength of recycled polymer concrete were improved by increasing amount of polyester resin and by optimizing the particle-size distribution of the microfillers. Besides, the results show the feasibility of developing a polymer concrete with excellent mechanical behavior.
1. Introduction Polymer concrete (PC) is a composite material which is composed of polymeric resins that act as binder materials of aggregates and microfillers. After the addition of different additives (catalysts and accelerators), the binders undergo polymerization resulting in a hardened composite. The primary difference, compared with cement-based concrete, apart from not containing hydrated cement, is that PC is stronger, more durable, and with lower maintenance requirements [1, 2]. However, portland cement can be used as microfiller or aggregate  in PC. Besides these advantages, this composite, which can reach mechanical strengths 45 times higher than cement-based concrete  keeping the modulus of elasticity in similar values , has good chemical resistance and water impermeability [6, 7]. For these reasons, PC is widely used in different applications of civil engineering [1, 8]. It has been used as a major component for the construction of box culverts, underground pipes, trench lines, industrial floors, also as bridge deck overlays,
and in reparation tasks of damaged cement-based concrete structures. In spite of these advantages, PC presents disadvantages that have limited its worldwide utilization. These PC disadvantages may be: expensive cost of resins used as binder agents, suitable precautions that should be applied to achieve a proper curing of PC, and need to use the high quality aggregates to produce PC, when it is compared with cementbased concrete. In order to reduce the high costs of competitive PC, together with recent environmental concern about wastes that end up in landfills, several researches [9, 10] have been conducted to analyze the properties of PC made with industrial byproducts and cement-based concrete residues acting as aggregates. Commercial epoxy resins and commercial unsaturated polyester resins, whose good results are widely known , can be found among the classic resins used as binder agents. Recently, plastic wastes and bottles from polyethylene terephthalate (PET) have been used for unsaturated polyester resins production, which were used as the binder agent to produce
The Scientific World Journal Table 1: Physical properties of binder used.
Viscosity Density (g/cm3 , 25∘ C) (Pa⋅s, 25∘ C) 1.10
Styrene content (%, 25∘ C)
Water absorption (%)
recycled PC [6, 9, 12]. The results of these investigations were very promising. They opened an important way to reduce costs and environmental pollution caused by wastes disposal. For their part, in order to achieve high mechanical performances by using expensive resins, high quality aggregates are commonly used. This optimum combination results in PC that fulfills such requirements [13, 14]. In this respect, a wide variety of materials are used, including quartz, silicates, gravel, limestone, calcareous, granite, clay, natural basalt, and calcium carbonate. Somewhat similar to the resin replacement, aggregates and microfillers have also been replaced by solid wastes from various industrial fields. Demolition materials from concrete and masonry wastes , residual glass from blasting operations , industry development and electrical production wastes such as fly ash or silica fume , crushed polymer concrete and mortar , rapid-cooled slag from the steel production process , or residual sands from foundry industries [19, 20] have been studied as mineral aggregates and microfillers in the production of recycled polymer concrete (RPC). These investigations concluded that it is feasible to produce high quality RPC based on recycled solid wastes and performances of resultant materials could be improved by optimizing different variables of the mixtures. Such variables were, in any case, aimed towards varying the ratios of resins : microfillers : aggregates used, the particlesize distributions of aggregates used, as well as their nature, and type of resins added to the mixtures. Focusing the interest in the case of recycled aggregates from concrete and PC, the obtained results were very encouraging. Generally, as the amount of binder increases, the void ratio in PC mixtures decreases, while compressive strength and flexural strength increase. Although this is affected not only by such variables but also by grading and mixture of microfillers and aggregates used [9, 15]. Besides these facts, as a gradual increase in the content of the recycled aggregate takes place, a reduction in the modulus of elasticity of the PC can also be seen . On the other hand, the use of aggregates from recycled PC has shown the feasibility of using them as a competitive alternative, compared with natural aggregates, producing only changes in mechanical strengths within 1% of significance statistic level . In the case of portland cementbased concrete there is a wide range of previous investigations related with the partial or complete substitution of coarse and fine natural aggregates by recycled aggregates from concrete [21–23]. Results of those studies generally concluded that the cement-based developed concretes with recycled aggregates offered less mechanical strengths and lower elastic modulus. Recently, the growing environmental awareness on the reuse of solid wastes from disused infrastructures, alongside the difficulties to obtain high-quality natural aggregates, leads to the study and incorporation of these waste materials as
PC components. In this research, the fundamental sources of aggregates are the replaced concrete sleepers or those whose manufacture has been faulty. Railway sleepers are essential elements in railroads; their main role is to distribute loads from the railway vehicles to the underlying ballast bed. Particularly, in the case of high-speed railroads, loads are very demanding. Therefore, materials that compose these elements should provide the maximum performance . In the case of concrete sleepers, the most used composition for their manufacture in Spain is siliceous aggregates, limestone, and basalt. Their mechanical properties are very suitable; consequently, they may provide an excellent source of high-quality recycled aggregates. From these considerations, this paper presents the results of experimental research on PC made with unsaturated polyester resin, microfillers, and recycled aggregates from crushing, cleaning, screening, and sieving replaced concrete sleepers or faulty ones. Furthermore, it also attempts to assess the mechanical properties of new PC, by varying the resin content, the nature of the recycled aggregate, and the particlesize distribution of microfillers blended.
2. Materials and Methods 2.1. Materials Used 2.1.1. Resin. Unsaturated orthophthalic polyester resin available as a commercial product HEGARDT H-76.1 was used to manufacture all mixtures developed in the present research. Table 1 shows the main physical properties of the used binder, according to the manufacturer. This polyester resin offers a low exothermic peak (200∘ C) and low volume shrinkage, therefore it is especially recommended for the production of PC. Methyl ethyl ketone peroxide (MEKP) in dimethyl phthalate (DMP) was used as initiator for this selected polyester resin.
2.1.2. Aggregates. Three different fine-size aggregates with a nominal maximum size of 4 mm, according to European Standard EN 12620:2009, were used: natural basalt (NBA), obtained from crushed basaltic rocks; recycled basalt (RBA), obtained from replaced and defective concrete sleepers; and recycled limestone (RLA) obtained following the same procedure that for RBA. The process used to recycle railway sleepers consisted of crushing the whole element, as indicated afterwards. Firstly, the sleeper was crushed. Secondly, the steel and iron particles were removed using a magnetic process. Thirdly, the resultant granular materials were screened to obtain well-graded aggregates. When this process was completed, the treated material was crushed again so as to produce the desired particle-size distribution, and air flow currents were applied to remove dusty particles. Finally, the resultant aggregates were cleaned with water and sieved. In spite of this complex treatment, mortar appeared attached to the particles at the end of the process. Absorption tests and frost/thaw cycle resistant tests were carried out to quantify the
The Scientific World Journal
3 Recycled basalt aggregates 120
100 80 60 40 20 0
Figure 1: Recycling railway sleepers process.
Figure 3: Basalt recycled aggregates gradation. Natural basalt aggregates
Recycled limestone aggregate
100 Passing (%)
100 80 60 40
80 60 40 20
Figure 4: Natural basalt aggregate gradation. Figure 2: Limestone recycled aggregate gradation. Table 2: Physical properties and chemical composition of the three microfillers used.
remaining mortar attached to the aggregates. Figure 1 shows a photograph of the process described. It should be noted that water absorption of RBA (8.7%) was higher than RLA (6%); this fact indicated that RBA had more attached mortar (from high resistant portland cement concrete) because of its rougher surface. In the frost/thaw cycle resistant tests (EN 14617-5:2012), RBA aggregate reduced its weight by 0.9% and RLA by 0.3%. These results were in accordance with those obtained in the absorption tests. For its part, density values were similar for all of the recycled aggregates (𝜌RBA = 2.58 g/cm3 and 𝜌RLA = 2.48 g/cm3 ). Different types of aggregates were used to analyze their influence in the PC mechanical performance depending on the origin and nature of them. Particle-size distributions of these aggregates were not considered since they are practically equal in size, as it can be seen in Figures 2, 3, and 4 in which aggregates gradation appears. 2.1.3. Microfillers. In order to enhance the bonding strength between resins and inorganic aggregates, three different microfillers from calcium carbonate (CaCO3 ) were used . Individual microfillers had the same origin, only the particlesize distributions were modified and, therefore, their bulk densities and moisture contents. Physical properties of the three microfillers: MF1 (maximum grain size of 500 𝜇m), MF2 (maximum grain size of 100 𝜇m), and MF3 (maximum grain size of 1 mm), are given in Table 2.
Type MF1 (CaCO3 ) MF2 (CaCO3 ) MF3 (CaCO3 )
Max. grain size (mm)
Bulk density (g/cm3 )
0.5 0.1 1
0.93 0.86 1.35
0.06 0.06 0.2
A comparison of the three different particle-size distributions is shown in Figure 5. This study blends the three individual microfillers for the production of PC with variations in the finest particles (